Study on Vacuum Roasting Pretreatment of Carbonaceous Gold Concentrates Based on Nonoxidation Technology

Carbonaceous gold ores are difficult to treat because of the “preg-robbing” by carbonaceous matters and locking by minerals. Roasting is the most commonly used method that is useful in dealing with carbonaceous gold ores. In this study, flotation gold concentrates containing sulfides and carbonaceous matters were investigated to ascertain the reaction process and the matters’ transformation characteristics in different temperatures by vacuum roasting pretreatment. Calcine and volatile condensates were characterized with several techniques. In the process of vacuum roasting, the main chemical reactions were decomposition reaction and carbothermic reduction reactions of sulfide ores, carbothermic reduction reactions of SiO2, and thermal decomposition reactions of organic carbon.-e bad effects of “preg-robbing” by carbonaceous matters were greatly weakened by the thermal decomposition and carbothermal reduction. -e gold locking minerals were mainly removed by reduction reactions. -e sulfides were removed in ways that did not produce SO2. -e removal of sulfur and carbonaceous matters during the vacuum roasting process was 95.83% and 65.38%, respectively. Direct cyanidation of the calcine extracted from 2.13% to 88.37% of the gold content with a vacuum degree of 10 Pa and roasting from 25°C to 1,200°C for 30min.


Introduction
With the depletion of oxide ores throughout the world, refractory gold ores are becoming of increasing importance to the mining industry [1]. Carbonaceous gold ores are important refractory gold ores in the world. In China, the accumulated resources of carbonaceous gold ores are 1,000 t, accounting for 8% of the gold resources and ranking second in the world [2][3][4]. erefore, the development and utilization of carbonaceous gold ores have gained considerable attention [5].
In carbonaceous gold ores, the following conditions are observed: (i) Natural gold is usually locked by minerals, such as sulfide (e.g., gold is occasionally embedded in the crystal center of pyrite with fine grain size [6]), silicate, and carbonate [1,7]. It is difficult to expose gold for contacting with a leaching solution through fine grinding alone. (ii) Some simple and organic carbons in carbonaceous gold ores can easily absorb dissolved gold during cyanide leaching, which is called "preg-robbing" and seriously affects leaching. (iii) Part of the organic carbon itself can lock gold, which makes the gold recovery more difficult [8].
ese factors make carbonaceous gold ores difficult to deal with. A small number of carbonaceous matters could have a significant impact on gold recovery. Riina Ahtiainen and others have found that the gold loss rate increased with the increase of carbonaceous matters' content in the carbonaceous gold ores. e gold loss rate was 29% when the carbonaceous matters' content was 0.01%, but when the carbon content was more than 10%, the gold was almost completely lost [9]. erefore, the key problem in improving the gold leaching rate is to solve the influence of carbonaceous matters. In order to eliminate or passivate the carbonaceous matters, the carbonaceous gold ores can be pretreated before cyanidation, by methods such as blanking, roasting, chlorination, or biooxidation [10]. Roasting is the oldest and still the most commonly used pretreatment method, which is applied to heat the sulfides or arsenide ores in the air to remove sulfur, arsenic, carbonaceous matters, or other volatiles through the processes of combustion [11,12]. In the earlier study, the flotation experiments were conducted as the pretreatment method to delete the effect of carbonaceous matters, while the leaching effects were terrible. en the conventional roasting experiments were conducted and the gold leaching rate had obviously improved but still did not reach the best. Considering the double refractory characteristic, the high carbon content of the sample, and the limitations on waste gas treatment, the focus of the later study was turned to the improvement of conventional roasting pretreatment technology [10].
Vacuum metallurgy technology has a good effect on improving metal recovery rate and shortening process flow in the field of minerals and metallurgy. e vacuum environment can meet the requirements of environmental protection, matters in the reaction system can be divided from the atmosphere, and the exchange of materials can be effectively controlled [13][14][15]. In the field of gold processing, vacuum technology is mainly used for the removal of arsenic and sulfur from arsenic-containing and sulfur-containing gold ores. e study found that, compared with the air and nitrogen atmosphere, the arsenic removal time in the vacuum was shorter, the temperature for arsenic removal was lower, and the arsenic removal rate was close to 98.97% at 1053.15 K and 3 h in the vacuum condition [16]. Many theoretical, technological, and equipment researches about vacuum technology have been carried out on the removal of arsenic from arsenic-bearing gold ore by vacuum method at the Technical University of Kazakhstan [17]. However, no relevant application of vacuum technology in the removal of carbon from carbonaceous gold ores has been found.
Carbothermal reduction technology is widely used in chemical and metallurgical industry, such as metal smelting, metal material preparation, lead-zinc oxide ore treatment, and other industrial productions. In recent years, the carbothermal reduction method has been applied to gold processing [18]. For example, based on the fluidized roasting coupling technology, the roasting process of reducing pyrolusite with carbonaceous gold ores was investigated. Corecovery of manganese from pyrolusite and gold from carbonaceous gold ores was achieved by this process. e results indicated that the optimum leaching efficiency of 99.31% for manganese and 97.43% for gold could be attained under the conditions that the mass ratio of carbonaceous gold ores to pyrolusite was 2 : 3, the coroasting temperature was 1073.15 K, and the roasting time was 30 min [19]. e experimental result showed that the carbonaceous matters in the carbonaceous gold ores can be utilized under proper conditions. Recently, studies found that carbothermal reduction can achieve good results under the vacuum condition. Yucheng Liu [20] investigated the mechanism of carbothermal reduction of indium ore under the vacuum condition.
e study found that the lower the system pressure was, the lower the initial reaction temperature of thermal decomposition of In 2 O 3 to In 2 O and In would be.
e Gibbs free energy in the reaction of InO and CO increases, and some side effects were difficult to occur. Luo Qi [21] have studied the vacuum carbothermal reduction characteristics of nickel laterite. e research showed that the vacuum system could improve the reduction efficiency of minerals at 973 K by changing the microstructure of most minerals, such as talc and nickel-bearing, and promote the thermal decomposition of the minerals.
In this study, the combination of vacuum metallurgy and carbothermal reduction technology was developed and used on the pretreatment of carbonaceous gold concentrates to synchronously solve the problem of minerals locking of gold and "preg-robbing" of carbonaceous and develop an environmentally friendly pretreatment process. e technology of vacuum roasting pretreatment has now obtained a Chinese national invention patent [22]. In this paper, the reactions process and the matters transformation characteristics in different temperature under the vacuum roasting pretreatment were studied in the present study. e variation characteristics of the calcine minerals compositions at different temperature stages and the volatile condensates were also analyzed to judge the reaction process.
e study led to a deeper understanding of the technology and made up for the deficiencies in the theoretical study of this technology.

Experimental
2.1. Materials. A 5 kg carbonaceous gold concentrate samples for this study were obtained from a gold factory in the Qinling Mountains, Shaanxi Province. e raw carbonaceous gold ore in the factory was pulped to 35% solids and floated in Denver Flotation Cell. e pulp was conditioned with copper sulfate. Sodium isoamyl xanthate and terpenic oil were the collector and foaming agents. After three flotation procedures, carbonaceous gold concentrates were obtained. e particle size of carbonaceous gold concentrates was 70% passing size of −75 μm. e results of the process mineralogical analysis of the raw sample are shown in Figures 1 and 2 and Tables 1-3.  Tables 1 and 2 show the chemical composition analysis and the mineral compositions of the raw sample. Figure 1 shows MLA images of the raw sample. Figure 2 shows the gold phase images of the raw sample. Table 3 presents the gold phase analysis results. Table 4 contains the carbon phase analysis results. e process mineralogical analysis results show that carbonaceous gold concentrate has a high quartz content of 72.34% and pyrite is the most abundant metal mineral at 6.50%. e minerals are mainly irregularly granular and have no fixed alignment except that calcite is in a state of aggregation. e carbon content is high, with total carbonaceous material content being 14%.
Gold phase analysis results show that gold exists in the form of natural gold with irregular shape and fine particle size less than 10 μm. e gold in Figure 2(a) is in the form of single gold. e phenomenon of gold being locked is serious. 65.35% of gold was locked by minerals, and the highest content of locking minerals was sulfides for 43.57%.

Experimental Procedure.
e flotation concentrates were washed several times with water and dried at 80°C in a drying oven; after that, samples were fully mixed. A 30 g of samples was put into a corundum porcelain boat and was placed in the center of the heating area of the quartz tube ( Figure 3). Heat from 25°C to the aimed temperature under 10 Pa vacuum degree and keep the aimed temperature for 30 min. e aimed temperatures were 600°C, 700°C, 800°C, 900°C, 1,000°C, 1,100°C, and 1,200°C. Every sample was cooled down to room temperature in vacuum environment after roasting, after which the weight was taken. With the limited capacity of the quartz tube, several roasting experiments were conducted under the same conditions, and the calcine was mixed to analyze and conduct leaching experiments under each set of conditions. Cyanidation tests were directly performed on 100 g after the vacuum roasting pretreatment processes. Leaching was performed at 35% solids by weight and the cyanide strength was maintained at 2 kg/t. e pulp was continuously stirred at a stirring speed of 300 r/min. e pH was maintained between 11 and 13 using CaO powder. e leaching time was 12 h. e gold content of cyanidation tailing was detected by the detection institution using Flame Atomic Absorption Method (TAS-900). In order to reduce the experimental error, the average gold leaching rate was obtained for 3 times using leaching tests.

Analysis and Characterization.
e process mineralogical analysis of the raw samples was performed by an FEI Mineral Liberation analyzer Model 250, equipped with a scanning electron microscope (FEI QUANTA 650) and energy spectrometer (EDAX APOLLO X). X-ray photoelectron spectroscopy (XPS) measurement was carried out on a ermo ESCALAB 250Xi device, using an Al Kα monochromatic X-ray source operated at 150 W and 15 keV. e pressure inside the analysis chamber was maintained below 1 × 10 −8 mbar. e emission angle is 60°, and the size of the analyzed area is 500 × 500 μm. e survey spectra were taken in the mode with analyzer pass energy 100 eV and energy step 1 eV. Detailed spectra of characteristic XPS lines were taken in the mode with analyzer pass energy 30 eV and energy step 0.01 eV. Energy shift was compensated by referencing all the spectra to a C1s signal taken as 284.8 eV which comes from the adventitious carbon with an aliphatic nature (sp3) and a characteristic signal at 284.8-285.0 eV. With the difference of sample exhibits in different environments and exposure time, calibration with C1s may have errors [23]. To avoid the influence of the probable errors on the result of XPS analysis, the sample composition test results, a large number of references, and XPS standard spectrum library were referenced to ensure the accuracy of the XPS analysis results. e volatile condensates were  characterized by X-ray diffraction (XRD) on an Xpert Pro MPD device and energy dispersive X-ray spectroscopy SEM-EDS on a TESCAN Vega3 device. Table 4 shows the results of the C phase analysis and S contents of the samples in different conditions. e S content in gold concentrates continuously decreased with the increase of temperature. Finally, it decreased by 95.83% when the temperature increased to 1,200°C compared with the original sample. Some yellow gas gradually appeared in the quartz tube at 500°C-600°C. e organic carbon content decreased by 8.48% compared with the original sample. e remaining 4.49% of organic carbon might be the reaction residue. e graphite content slightly decreased at 800°C because of the redox consumption [24], while it increased at 1,200°C    Journal of Chemistry 5

Analysis of Sample Quality Changes.
because of the fact that thermal decomposition of organic carbon could form graphite at a high temperature. e decomposition reaction reduced the carbonate content to 800°C. As the temperature continues to rise, the carbonate content would be increased, and this might be related to the ash produced by the thermal decomposition of organic carbon. Table 5 shows the results of sample quality variation at different temperatures. e mass loss of samples gradually increased with the increase of temperature, and the increase of mass loss changed obviously at 800°C and reached the maximum of 37.80% at 1,200°C. Figure 4 shows the XPS analysis of the total spectrum of samples at different conditions. As shown in Figure 4, the characteristic peak of the elements in the sample had changed obviously after vacuum roasting. e evident change occurred at 1,200°C with the absorption peak strength of Fe 2p and C 1s weakened, but Si 2p enhanced. e binding energy of S 2p, Fe 2p, and Si 2p was slightly offset compared with untreated samples when roasted at 800°C (Table 6), but it immensely changed at 1,200°C with S 2p and Fe 2p, respectively, having only one binding energy peak at 173.54 and 710.04 eV and Si 2p having a new binding energy peak at 101.24 eV. e results showed that the existing form of some elements like S, Fe, and Si was changed obviously at 1,200°C [25]. e narrow peak scanning analysis was conducted on the main elements under different conditions to make a clearer analysis of the reaction process. Figure 5 shows the narrow peak scanning analysis of S 2p, Fe 2p, Si 2p, and O 1 s.

XPS Analysis of Calcine.
It can be seen from Figure 5 and the mineral compositions of the sample ( Table 2) that S 2p mainly existed in the form of metal sulfate and sulfide in the untreated samples. e corresponding peak value of S 2p gradually decreased with the increase of roasting temperature, and it nearly disappeared at 1,200°C. e result shows that the S element was effectively reduced or removed in the reaction process, while whether there was any remaining S-containing substance needs further verification.
In Fe 2p spectrum, the peak values of 711.70 eV and 725.66 eV corresponded to Fe-O bond in the untreated samples [26], and the peak of binding energy in other positions was not obvious to judge the existence state of Fe. e peak of Fe 2p decreased gradually with the increase of roasting temperature, and it nearly disappeared at 1,200°C. It can be seen that an obvious chemical reaction took place in   Si 2p spectrum seemed to be very similar under the untreated conditions and was treated at 800°C conditions, which showed that the existence morphology of Si had not changed obviously by vacuum roasting at 800°C [27]. At 1,200°C, there was an obvious peak at the binding energy of  101.24 eV, which indicated that some reactions happened on Si-containing materials and the existence form might have changed. In order to observe the final reaction products of Si, the spectra deconvolution of Si 2p was conducted ( Figure 6). Finally, combined with the mineral compositions of the sample (Table 2), Si had three existence states of SiO 2 , aluminosilicate, and SiC (the corresponding binding energy was 103.92eV, 101.93 eV, and 101.29eV). SiO 2 and aluminosilicate were the substances in the original sample. SiC [28,29] was a new product, which was probably due to a reaction between C and a siliceous material. e spectra characteristics of O 1s looked similar at the three treatment conditions. With the main presence states of oxygen being stable forms, the corresponding substance states of oxygen had little change. e spectra deconvolution of O 1s at 1,200°C was conducted ( Figure 6) to analyze the final products. Two peaks at 532.93 eV and 531.84 eV corresponded to existence states of O (SiO 2 and organic C-O) [27]. Other existence states of O were not found, possibly because the content was too low to be detected.
In order to study the change of carbonaceous matters in the reaction process, the spectra deconvolution of C 1s was conducted ( Figure 7). As it can be seen from Figure 7, the peaks of C 1s were at 283.99, 284.8, 285.54, 286.55, and 289.07 eV in the untreated samples, but it changed at 800°C and disappeared at the peak at 289.07 eV, and the position of other peaks did not change much. At 1,200°C, there were two new peaks appearing at 289.70 eV and 283.41 eV. According to the results of the sample composition and the standard spectrum library of the electron binding energy of C, it can be inferred that the corresponding substances at 289.07 eV and 289.70 eV were metal carbonate [30,31], the corresponding substances were C-O bonds substances (organic carbon) at 285.54 eV [32], the binding energy at 286.55 eV corresponded to C � O bonds substances (organic carbon), the binding energy at 283.99 eV corresponded to C � C carbon substances (graphite) [33], and the binding energy at 283.41 eV might correspond to SiC, which might be the product of new reaction like carbothermic reduction reaction in the process [32]. It was worth noting that carbonate in the samples was not detected at 800°C, which indicates that the carbonates might have been decomposed, but it appeared at 1,200°C, indicating that the reaction might produce new carbonate; this result was consistent with the previous phase analysis result of carbon.

SEM-EDS and XRD Analysis of Volatile Condensates.
In the vacuum roasting process, volatile condensates were different at different temperatures. At 800°C, a small amount of yellow condensate was found in the quartz tube, but it was too less to be detected. erefore, the volatile condensate at 1,200°C was detected and analyzed. Figure 8 shows the photo of volatile condensates in the quartz tube wall at 1,200°C. Figure 9 shows the results of SEM-EDS analysis of volatile condensates.
As shown in Figures 9(a)-9(g), evident differences could be found between the morphology of volatile condensates. e main elements of volatile condensates were Si, S, and O, whereas Na, Mg, P, K, and Zn were few. A large amount of rod-like structure matter might correspond to SiO 2 (Figure 9(a)). e matter in Figure 9(b) looked compact and it contained a large amount of Si and S and a small amount of MgO and K 2 O. In Figure 9(c), the materials with heterogeneous spherical structure were mainly SiS 2 and minimal ZnO. In Figure 9(d), with the little content of other elements, the flake shape matter seemed to correspond to Si. In Figure 9(e), ZnS was the main matter of the uniformly dispersed sphere. e matter in Figure 9(f ) seemed to be similar to Figure 9(d), the morphology was cluster-like and rich, which might be Si. As shown in Figure 9(g), the interface of the product was flat, and the corresponding substances were Si and ZnO. Figure 10 presents the XRD analysis of the volatile condensates at 1,200°C. e diagram showed that the volatile condensates were mainly composed of S, Si, SiO 2 , SiS 2 , ZnO, ZnS, and MgO. Under the vacuum condition, the S in the volatile condensates came from the decomposition reaction of FeS 2 . e Si and SiO 2 condensates might be the intermediate product of the carbothermal reduction reaction of SiO 2 [33]. MgO might be produced by the decomposition reaction of dolomite. SiS 2 condensed on the tube wall might be formed through the contact reaction of Si and sulfur gas [34]. e ZnS and ZnO condensates might be produced by the volatilization and other unknown reactions of ZnS, respectively. Table 7 shows the gold phase analysis of calcine at 1,200°C. Compared with the results of untreated samples in Table 3, the content of exposed and semiexposed gold increased from 34.65% to 57.56%; this result showed that the gold liberation had been improved and gold leaching would be easier than the raw sample.

Analysis of Gold Dissociation Effect.
e content of sulfides-locked gold had greatly reduced from 43.57% to 5.57%, which showed that the vacuum roasting could effectively solve the gold locking problem by sulfides.

3.4.1.
e ermodynamic Analysis of Main Minerals. e main chemical reactions and the whole reaction process of vacuum roasting pretreatment of carbonaceous gold concentrate were obtained by combining the analysis results of calcine and volatile condensates. e main chemical reactions were decomposition reaction (equation (1)) and carbothermic reduction reactions (equations (2) and (3)) of pyrite [35], carbothermic reduction reactions of SiO 2 (equations (4) and (5)) [36], and thermal decomposition reaction of organic carbon (equation (6)) [37,38]. e results of thermodynamic analysis of the main chemical reactions in the vacuum roasting pretreatment processes are shown in Figure 11.

12
Journal of Chemistry CaMg CO 3 2 CaO + CO 2(g) ⟶ e main reaction process of the vacuum roasting pretreatment process is as follows: (1) e Reactions of FeS 2 . Under vacuum condition, the decomposition reaction of FeS 2 could take place at 513°C, and the temperature of carbothermic reduction reactions is 470°C and 731°C, respectively. erefore, the carbothermic reduction reactions might take place preferentially in actual reactions. During the roasting experiment, yellow gas was produced at 500~600°C, which gradually condenses and eventually becomes sulfur during the cooling process.
e decomposition reaction of FeS 2 was verified. erefore, both the decomposition reaction and the carbothermic reduction reaction of FeS 2 could take place in the range of experimental temperature.
(2) e Reactions of SiO 2 . e carbothermal reductions of SiO 2 in vacuum roasting pretreatment process were very complicated. us, the thermodynamic analysis only listed the reactions with significant products in the experimental process [39]. e first carbothermal reduction reaction (equation (4)  confirmed with the SiC that appeared in calcine at 1,200°C in the XPS analysis part. e second reaction (equation (5)) could take place at 1155°C. e silicon in the product was in a gaseous state firstly and then it condensed on the tube wall, which showed how the silicon in the condensate came from. erefore, the carbothermal reduction of SiO 2 could take place in the range of experimental temperature, and the treatment of SiO 2 was effective. e carbonaceous matter was grouped by elemental carbon and organic carbon in the original sample. In theory, all of the carbothermal reduction reactions (equations (2)-(5)) of elemental carbon could take place, while with the small initial content of elemental carbon, only two lower temperature reactions (equations (2) and (3)) might take place in real experiments. e thermal decomposition and dehydrogenation reactions (equation (6)) might be the main reactions of organic carbon. e thermal decomposition reaction was a seriously mass-weightless process, which might end at about 900-1,000°C. e dehydrogenation reaction was the second reaction stage of organic carbon, which continuously produced carbon. And this was also the reason for the increase of graphite content in calcine at 1,200°C. is elemental carbon produced by organic carbon could continue to participate in the reaction of other substances, such as the carbothermal reduction reaction (equations (4) and (5)). (4) Reactions of Other Substances. Carbonates content decreased first and then increased during the pretreatment process, which was related to the decomposition and formation reactions of carbonates (equations (7)- (9) (10)) which was generated in the thermal decomposition and dehydrogenation reactions of organic carbon at 500°C after its dehydration reaction. With the low content, it was difficult to analyze the late reactions of these substances. In addition to the reactions of minerals occurring in the heating region, a variety of products could be seen in the condensation region, which might be products of the reactions of the original substances or secondary products of these reactions. erefore, these complex reactions in the vacuum roasting pretreatment process were still needed to be further studied.

e Mechanism Diagram of Major
Reactions. e main factors affecting gold leaching could be effectively improved by the vacuum roasting pretreatment method. Bellow 800°C, the main reactions were dehydration reactions of water-bearing materials, decomposition reactions and carbothermic reduction reactions of sulfides ores, and thermal decomposition reactions of organic carbon. Above 800°C, the main reactions were carbothermic reduction reactions of SiO 2 , thermal decomposition reactions of organic carbon, and some complex reactions of other prime matters or their secondary reaction. Figure 12 only shows the main reaction process of sulfides ore and carbonaceous matters to make the reaction process clearer.

Analysis of Leaching Effect.
e gold leaching results under different pretreatment temperatures are shown in Figure 13. e results showed that the gold leaching rate gradually increased with the increase of temperature under the vacuum roasting condition; it increased from 2.13% to 88.37% after pretreatment at 1,200°C. Combined with Table 4 and Figure 13, the gold leaching rate was low when the roasting temperature is less than 800°C, while the organic carbon content was high (Table 4). With the temperature increase after 800°C, the organic carbon content significantly decreased, whereas the gold leaching rate evidently increased. is finding showed that organic carbon was the main factor affecting the gold leaching rate in the carbonaceous gold concentrates.
It is worth noting that the exposed and semiexposed gold increased to 57.56% after roasting at 1,200°C, but the gold leaching rate reached 88.37% finally. e result suggested that some of the locking gold was also leached. is might be due to the fact that the locking in the raw samples was broken. e locking did not completely abolish finally; this might be due to the new secondary locking produced by some reactions. However, the secondary locking might not be as tight as the original locking after a series of reactions and might leach more easily during the leaching process.

Discussion
e vacuum roasting pretreatment technology increased the gold recovery by solving the problems of "preg-robbing" and gold-locked. e gold leaching rate was immensely improved with vacuum roasting pretreatment at 1,200°C; however, there was still 11.63% of gold being lost; this part of the gold loss was a mystery and needs further study to get the ideal gold leaching rate [40]. at is to say, the fundamental reason why the gold was difficult to be recovered needed to be further studied. It was of great indicative significance to the selection of the pretreatment process for the same kind of carbonaceous gold ore, and it could also explain why the conventional roasting pretreatment and preferential flotation of carbonaceous matters cannot achieve good results. It is interesting that a large number of volatile condensates like elemental Si and S were produced during the vacuum roasting pretreatment process. e variation characteristics of condensate at different temperatures and whether they were available or not were worth studying; it was also an important aspect of maximizing the utilization of samples. e recovery of condensation was not easy due to the immaturity of test equipment in the present research. Improving the experimental equipment for more scientific recovery of volatile condensates is necessary for future research.

Conclusions
A good effect with the gold leaching rate increase from 2.13% to 88.37% was obtained with the vacuum degree of 10 Pa and the temperature of 1,200°C for 30 minutes. e removal of sulfur and carbonaceous matters during the vacuum roasting process was 95.83% and 65.38%, respectively. e content of exposed and semiexposed gold increased from 34.65% to 57.56%, which was beneficial to the gold leaching.
In the vacuum roasting pretreatment process of carbonaceous gold concentrate ores, the effect of temperature was obvious, and the increase of temperature was conducive to the carbothermal reduction reactions and the thermal decomposition of organic carbon. e pretreatment effects increased after 800°C, at which the thermal decomposition of organic carbon was gradually completed. Some of the carbonaceous matters contained in the carbonaceous gold ores became the reductant to participate in the reaction, which not only realized the recovery of the target minerals but also realized the purpose of waste utilization. e recovery of gold could be effectively improved by removing the carbonaceous matters and reducing the gold locking of sulfide ores. With the S element transformed into S 2 instead of SO 2 , the cost of waste gas treatment could be reduced. is research provides a new idea for the comprehensive utilization of carbonaceous materials and the development of a roasting pretreatment method for carbonaceous gold ore.

Data Availability
e data used to support the findings of this study are included within the article.

Conflicts of Interest
e authors declare that they have no conflicts of interest.